Aug 6, 2010 - and Comparison with Continuously Graded Antireflection Coatings. Martin F. .... quarterwave coating, by properly optimizing the thicknesses.
Applied Physics Express 3 (2010) 082502
Performance of Antireflection Coatings Consisting of Multiple Discrete Layers and Comparison with Continuously Graded Antireflection Coatings Martin F. Schubert, David J. Poxson, Frank W. Mont, Jong Kyu Kim1 , and E. Fred Schubert Department of Physics, Applied Physics, and Astronomy, Department of Electrical, Computer, and Systems Engineering, Rensselaer Nanotechnology Center, Rensselaer Polytechnic Institute, Troy, NY 12180, U.S.A. 1 Department of Materials Science and Engineering, Pohang University of Science and Technology, Pohang 790-784, Korea Received June 11, 2010; accepted July 14, 2010; published online August 6, 2010 The performance of discrete multilayer and continuously graded antireflection coatings for omnidirectional broadband applications are compared. It is shown that in practical cases where refractive index choices are constrained, discrete antireflection coatings can surpass the performance of continuously graded coatings by taking advantage of interference effects, which continuously graded coatings are expressly designed to avoid. A four-layer antireflection coating designed using a genetic algorithm is fabricated, and is experimentally shown to have reflectivity lower than what is achievable for continuously graded designs. # 2010 The Japan Society of Applied Physics DOI: 10.1143/APEX.3.082502
esigns for broadband omnidirectional antireﬂection (AR) coatings are generally motivated by the hypothesis that smooth and gradual variation of the refractive index over an extended distance will produce the best possible AR characteristics. AR coatings with refractive index proﬁles that vary continuously from the substrate refractive index to the ambient value are known to have excellent performance. However, in virtually all applications, the refractive index of the AR coating is constrained by the availability of materials with refractive indices matching the substrate and the ambient. Nevertheless, experimentally realized broadband omnidirectional AR coatings have used refractive index proﬁles intended to approximate continuous grading. Here it is shown that, contrary to common assumption, AR coatings consisting of only a few discrete layers can signiﬁcantly outperform AR coatings of any continuously graded proﬁle over a broad range of wavelengths and incident angles. Even compared with inﬁnitely thick continuously graded AR coatings, the discrete multi-layer approach has a lower angle- and wavelength-averaged reﬂectivity. The pursuit of low-reﬂectivity coatings has fascinated researchers for more than a century.1–9) While it is straightforward to attain low reﬂectivity for normal incidence and a narrow wavelength range, achieving omnidirectional and broadband AR characteristics is far more challenging, but also more relevant for many applications. In 1880, Lord Raleigh analyzed reﬂections of waves from graded interfaces between two dissimilar media, and realized that ‘‘the transition may be so gradual that no sensible reﬂection would ensue’’.1) That is, for an inﬁnitely thick, continuously graded AR coating, Fresnel reﬂectivity approaches zero. Signiﬁcant research has focused on ﬁnding refractive index proﬁles which minimize reﬂection for a given AR coating thickness. A linear proﬁle is a reasonable starting point, but other proﬁles, such as the quintic proﬁle, have been found to give superior performance.3,4) Recently, oblique-angle deposition has been used to demonstrate nanoporous ﬁlms with a refractive index approaching that of air.9,10) These nanoporous ﬁlms are stable, showing no signs of deterioration over time or in response to aqueous environments. Besides allowing very low refractive index values, oblique-angle deposition and
Present address: Micron Technology Inc., Boise, ID 83716, U.S.A.
other techniques can be used to precisely tune the refractive index within a broad range by varying a material’s porosity.11,12) In principle, this combination enables AR coatings in which the refractive index is continuously graded. However, a fundamental limitation prevents implementation of true continuously graded air-ambient AR coatings matching Raleigh’s description: there exist gaps in the range of attainable refractive indices for transparent materials. For example, while refractive indices as low as 1.05 have been reported,9) values below this have not been reached, though they would be required for a true continuous AR coating where air is the ambient medium. In addition, transparent materials generally are not able to match the refractive index of an absorbing substrate, because absorbing materials have a complex refractive index whereas for transparent materials the refractive index is necessarily real. Thus, in the vast majority of practical applications, it is simply not possible to realize a graded AR coating as envisioned by Rayleigh, because portions of the required range of refractive index values are unavailable. One might suppose that an inﬁnitely thick, continuous graded-refractive-index approach is still the best option, despite unavoidable discontinuities in refractive index. Following this assumption, experimentally realized AR coatings are frequently intended to approximate continuous proﬁles.2,6–9) In this paper, however, we demonstrate that such coatings are, in fact, not the optimum for minimum angle-averaged and wavelength-averaged reﬂectivity for virtually all practical cases. We show that discrete multilayer coatings enable reﬂectivity far below values attainable by continuously graded coatings. Speciﬁcally, we show that interference of light — a phenomenon which is expressly avoided in continuously graded AR coatings — enables discrete multilayer coatings to deliver superior performance, particularly for broadband and omnidirectional applications. Approximating our step-graded refractive index proﬁle with a continuously graded proﬁle has been conﬁrmed to worsen the reﬂection properties of the AR coating, i.e., the interference eﬀects that continuously graded coatings expressly avoid, are weakened. This result is relevant to virtually all thin-ﬁlm coatings that have practical uses in photonics applications. Speciﬁcally, it applies to common components such as solar cells, sensors, detectors, lenses, and solid-state lighting devices. We consider light incident from a low-refractive-index ambient upon a high-refractive-
# 2010 The Japan Society of Applied Physics
Appl. Phys. Express 3 (2010) 082502
M. F. Schubert et al.
Fig. 1. Calculated wavelength-averaged reflectivity as a function of angle for linearly graded and quintic refractive-index profiles at 40 and normal incidence. Substrate refractive index is 4.0, the ambient index is 1.0, and the AR coating refractive index is limited to values between 3.0 and 1.1.
Fig. 2. Calculated angle- and wavelength-averaged reflectivity of an AR coating with a continuously graded quintic profile as a function of the coating thickness. Also shown is the averaged reflectivity of a discrete four-layer AR coating with thickness of approximately 700 nm. The discrete multilayer coating outperforms the continuously graded quintic profile for any thickness of the quintic coating.
index substrate. In the limit of a transparent, inﬁnitely thick, continuously graded AR coating, the reﬂection coeﬃcient is R ¼ 1 ð1 R1 Þð1 R2 Þ=ð1 R1 R2 ), where R1 and R2 are the angle- and wavelength-dependent reﬂection coeﬃcients, at the interfaces between (1) the ambient and the adjoining material of the AR coating, and (2) the substrate and the adjoining material of the AR coating, respectively. When these interfacial regions are also continuously graded, then the total reﬂection coeﬃcient will be zero. However, in cases where perfect refractive index matching is not possible, the discontinuity in refractive indices results in unavoidable reﬂections. The calculation of a wide variety of continuously graded proﬁles reveals that all of them asymptotically approach the reﬂection values shown for an inﬁnitely thick coating. Figure 1 shows the reﬂection coeﬃcient for a linearly-graded and quintic AR coating without perfect refractive index matching, and demonstrates that even in the limit of inﬁnitely thick graded-index coatings, there is a limiting value of the reﬂectivity which is independent of the functional form of the refractive index proﬁle. To demonstrate the high performance of optimized multilayer AR coatings, we consider light incident from air upon silicon, with the requirement that the AR coating be composed of nanoporous SiO2 and mixed SiO2 /TiO2 . We limit the porosity of SiO2 to 80%, which yields a refractive index around 1.1. We include all incident angles (0 – 90 ) and wavelengths between 400 and 1600 nm, and material dispersion is taken into account. Designing such multilayer AR coatings requires care, as the conﬁguration space of a multilayer AR coating has many local minima for reﬂection, and makes ﬁnding the true optimum AR coating a challenge. To design optimized multilayer AR coatings, we use a genetic algorithm, which prevents capture within local minima and is well suited to the design of optical coatings.13,14) Figure 2 shows the calculated wavelength- and angleaveraged reﬂection coeﬃcient as a function of thickness for a continuously graded quintic AR coating, and also shows
the performance of a 700-nm-thick four-layer AR coating designed to minimize the reﬂection coeﬃcient optimized over all wavelengths and angles. The results demonstrate the superiority of discrete multilayer coatings: An AR coating consisting of four discrete layers outperforms the continuously-graded quintic proﬁle AR coating for any thickness of the quintic coating. As the thickness becomes large, the averaged reﬂection coeﬃcient of the quintic AR coating approaches 13.59% for the transverse electric (TE) polarization, compared to 8.86% for the four-layer design. For transverse magnetic (TM) polarization, continuous grading yields 10.76% average reﬂection compared to 8.60% for the four-layer design. As mentioned earlier, in the limit of inﬁnite thickness all continuously graded AR coatings have identical performance, and therefore the optimized fourlayer design is superior to any conceivable continuously graded AR coating. Compared to the optimized four-layer design, the angle- and wavelength-averaged reﬂection coeﬃcient of an inﬁnitely-thick continuously graded AR coating is a remarkable 53 and 25% higher, respectively, for TE and TM polarizations. The four-layer AR coating is experimentally realized using co-sputtering for TiO2 /SiO2 layers, and oblique-angle deposition for nanoporous SiO2 layers. An scanning electron microscopy (SEM) image of the AR coating along with layer speciﬁcations is shown in Fig. 3. Layers of the AR coating are fabricated by co-sputtering of TiO2 /SiO2 and obliqueangle deposition of SiO2 using e-beam evaporation. Deposition angles for the nanoporous SiO2 are 85 and 60 for the 80 and 30% porous layers, respectively.11) Film thicknesses and refractive indices are characterized using variable angle spectroscopic ellipsometry. The porosity of a material is determined from the measured refractive index and a linear volume approximation in conjunction with an analytic expression for porosity as a function of deposition angle.11,12) The reﬂection coeﬃcient is measured as a function of angle using a broadband white light source and an optical spectrum analyzer.
# 2010 The Japan Society of Applied Physics
Appl. Phys. Express 3 (2010) 082502
M. F. Schubert et al.
Fig. 3. SEM image of the four-layer AR coating on a silicon substrate, shown with layer composition, thickness, and refractive index data. The refractive index is given at a wavelength of 485 nm.
diﬀerent interfaces. Just as in a ‘‘perfect’’ normal incidence quarterwave coating, by properly optimizing the thicknesses and refractive index contrasts of a discrete multi-layer AR coating will result in destructive interference for reﬂected light, and therefore low reﬂection coeﬃcient. For broadband (400 –1600 nm) and omnidirectional (0 – 90 ) AR coatings, this is highly surprising since one would expect that any interference eﬀects over a wide range of wavelengths and angles will average out. High performance is achieved by taking advantage of the very phenomenon that continuous AR coatings are speciﬁcally designed to eliminate. Therefore, only by discarding the continuous AR coating proﬁles as a starting point can performance of an AR coating be truly maximized. In summary, we have shown that the performance of continuously-graded AR coatings is fundamentally limited in virtually all practical cases where perfect index matching is not available. Further, it is theoretically demonstrated that discrete multilayer AR coatings can outperform continuously-graded AR coatings, by taking advantage of interference eﬀects arising from reﬂections within the coating — something which is expressly avoided in continuouslygraded designs. Using a genetic algorithm, an optimized a four-layer coating is demonstrated which oﬀers substantially lower reﬂectivity than even a hypothetical, inﬁnitely thick continuously graded coating. The broadband and omnidirectional reﬂection characteristics of an experimentally realized four-layer (TiO2 /SiO2 )/nanoporous SiO2 coating are in excellent agreement with theory. Acknowledgments This material is based upon work supported by the National Science Foundation under grant number DMR-0642573 and by NYSTAR under contact number C070119. The authors also gratefully acknowledge support by Samsung Electro-Mechanics, Sandia National Laboratories, Department of Energy, Department of Defense, Magnolia Optics, Crystal IS, Troy Research Corporation, and New York State.
Fig. 4. Calculated and measured angle- and wavelength-averaged reflectivity of the four-layer AR coating on a silicon substrate.
Figure 4 shows both calculated and measured reﬂectivity as a function of wavelength and incident angle for TE and TM polarization for the four-layer AR coating, and reveals local minima in reﬂectivity that are indicative of the interference which allow performance beyond the level of continuously-graded coatings. Experiment and calculation show excellent agreement. The measured average reﬂectivity between 10 and 80 and between 400 and 1600 nm is 5.29 and 4.63% for TE and TM polarization, which are very close to the calculated values of 4.93 and 4.32%, and to our knowledge, are the lowest values ever reported. The underlying reason that this four-layer AR coating outperforms even an inﬁnitely thick continuously graded coating is found in the interference of light reﬂected at
1) 2) 3) 4) 5) 6) 7) 8) 9) 10) 11) 12) 13) 14)
J. S. Rayleigh: Proc. London Math. Soc. 11 (1880) 51. M. J. Minot: J. Opt. Soc. Am. 67 (1977) 1046. W. H. Southwell: Opt. Lett. 8 (1983) 584. J. A. Dobrowolski, D. Poitras, P. Ma, H. Vakil, and M. Acree: Appl. Opt. 41 (2002) 3075. D. Poitras and J. A. Dobrowolski: Appl. Opt. 43 (2004) 1286. S. R. Kennedy and M. J. Brett: Appl. Opt. 42 (2003) 4573. M. Chen, H.-C. Chang, A. S. P. Chang, S.-Y. Lin, J. Q. Xi, and E. F. Schubert: Appl. Opt. 46 (2007) 6533. C. H. Chang, P. Yu, and C. S. Yang: Appl. Phys. Lett. 94 (2009) 051114. J.-Q. Xi, M. F. Schubert, J. K. Kim, E. F. Schubert, M. Chen, S.-Y. Lin, W. Liu, and J. A. Smart: Nat. Photonics 1 (2007) 176. J.-Q. Xi, J. K. Kim, E. F. Schubert, D. Ye, T.-M. Lu, and S.-Y. Lin: Opt. Lett. 31 (2006) 601. D. J. Poxson, F. W. Mont, M. F. Schubert, J. K. Kim, and E. F. Schubert: Appl. Phys. Lett. 93 (2008) 101914. W. H. Southwell: Appl. Opt. 24 (1985) 457. M. F. Schubert, F. W. Mont, S. Chhajed, D. J. Poxson, J. K. Kim, and E. F. Schubert: Opt. Express 16 (2008) 5290. D. J. Poxson, M. F. Schubert, F. W. Mont, E. F. Schubert, and J. K. Kim: Opt. Lett. 34 (2009) 728.
# 2010 The Japan Society of Applied Physics